iMedPub Journals 2017 http://www.imedpub.com Journal of Waste Recycling Vol.2 No.2:5
Isolation and Characterization of the Mineral Contreras M1*, 1,2 1 Phases in Ilmenite Ore: Optimization of the Gázquez J and Bolívar JP 1 Department of Applied Physics, Faculty TiO2 Pigment Process of Experimental Sciences, University of Huelva, Campus de Excelencia Internacional del Mar (CEIMAR), Huelva, Spain Abstract 2 Departament of Applied Physics, Escuela Superior de Ingeniería, Puerto Real,
The TiO2 production by the sulphate route uses ilmenite as raw material, which Cádiz, Spain is initially milled and dissolved by adding concentrated sulphuric acid (98%). A significant fraction of the original raw material (about 10-15%) cannot be dissolved in the digestion step. In order to recovery the titanium (rutile form) *Corresponding author: and other economic minerals during the digestion stay, was carried out a deep Manuel Contreras Llanes characterization of the used raw material in relation to several parameters, such as the elemental composition (major and trace elements), mineralogy, [email protected] microscopic morphology and physical composition. Therefore, the main goal of this work has been to separate and to analyse the minerals contained in the raw Department of Applied Physics, Faculty of material in order to isolate the potentially dangerous and economics minerals Experimental Sciences, University of Huelva, prior to the industrial process. The main conclusion the study was that the raw Campus de Excelencia Internacional del Mar, material is mainly composed of ilmenite and its alteration products (ilmenite Huelva, Spain. unchanged, leached ilmenite, pseudorutile, leached pseudorutile and rutile), produced by weathering of the original ilmenite, and containing small amounts Tel: +34959219793 of other minerals (monazite, spinel, quartz and zircon). According to this, a near total isolation of each mineral is very complex, but a high percent of them can be recovery by optimizing the industrial process. In addition, the economical impurities isolated can be commercial. Likewise, this fact could be reduced the Citation: Contreras M, Gázquez J, Bolívar JP (2017) Isolation and potential environmental impact of the TiO2 industries via sulphate by reducing the waste production. Characterization of the Mineral Phases in Ilmenite Ore: Optimization of the TiO2 Keywords: Ilmenite; TiO2 industries; Magnetic mineral separation; Particle Pigment Process. J Waste Recycl Vol.2 morphology; Textural constraints No.2:5
Received: September 15, 2017; Accepted: September 25, 2017; Published: September 30, 2017
structure. In addition, leucoxene (Fe O ·nTiO ) , is an oxidation Introduction 2 3 2 product of ilmenite which it is composed of finely crystalline In opposition of the popular belief, the most widely used titanium rutile. Other less common titanium oxide-bearing minerals are product is not the titanium metal and alloys, but rather is the pseudobrookite (Fe2TiO5), perovskite (CaTiO3), geikielite ((Mg,Fe) titanium dioxide (TiO ) pigment. This pigment provides whiteness 2 TiO3), pyrophanite (MnTiO3)  and the only silicate mineral with and opacity to a vast range of everyday products from coatings titanium as a major component is titanite (known as sphene and plastics, to inks and even as flux in glass manufacture, filler in (TiSiO5). Ilmenite is the most important economic mineral from paper, rubber industries , cosmetics and food. Annually more which TiO2 is extracted; due to the content of TiO2 is about 50% than 4.5 million tons of TiO2 are produced worldwide  and only and it is widely found. Despite that rutile, which is the richest about 4-5% is used to produce metallic titanium . Titanium is form of TiO2 (93-96% TiO2) occurring naturally but is not so basically found in nature as ilmenite ore (FeTiO3) either as a rock often found in deposits valid for commercial use. Finally can be or as sand, rutile, anatase and brookite, which although they all found as leucoxene (Fe2O3·nTiO2), a natural alteration product have the same formula (TiO2), but differing in their crystalline of ilmenite, containing often more than 65% TiO2 . More
© Under License of Creative Commons Attribution 3.0 License | This article is available in: http://www.imedpub.com/resources-recycling-and-waste-management/ 1 2017 Journal of Waste Recycling Vol.2 No.2:5 than half of the world’s titanium production is obtained from Materials and Methods ilmenite and rutile in shoreline placer deposits in Australia, South Africa, USA, India and Sri Lanka. Magmatic ilmenite deposits in Materials Canada, Norway, Finland and USA supply most of the remainder. The samples of raw material (“commercial ilmenite named The magmatic deposits yield ilmenite with a TiO2 content of 35- ILUKA”) were provided for use in this study by the titanium 40%, whereas the shoreline placer deposits provide ilmenite of dioxide production plant 12 km from the city of Huelva. Five higher TiO2 content, including altered ilmenite (60-75% TiO2), sampling campaigns were organised during a period of 1 leucoxene (76-90% TiO2) and rutile (95% TiO2) . On the other month, taking place every 6 days. The objective was to analyse hand, in alluvial sediments, ilmenite alters and Fe is partially the possible temporal variability in the characteristics of the leached in a continuous process going to pseudorutile (Fe2Ti3O9) materials, and to obtain representative samples to be used in the and leucoxene . For that reason, titanium and iron content new manufactured materials. After collection, the raw materials in the ilmenite may vary significantly, as it can be present in its were dried at 105°C. primary stoichiometric form (FeTiO ) or as weathered ilmenites 3 Methods and mixtures of both types. The weathered ilmenite is the result from the oxidation and partial dissolution by ground The identification of the mineral phases was performed by the water of the iron. In this sense, the progressive removal of this XRD technique (X-ray diffraction) in a Bruker diffractometer iron by leaching; and the relative increase in the concentration (model D8 Advance), using Cu Kα radiation operating at a current of 30 mA, and a voltage of 40 kV. Data were recorded in the 5–70° of impurity elements alters the original ilmenite . The TiO2 content can even exceed the 60% when the ore is altered to 2 Ө range (step size 0.019736° and 0.5 s duration for each step). leucoxene, which is a mixture of rutile or anatase amorphous According the mineralogical composition of the raw material was
TiO2 and iron oxides. In addition, ilmenite usually contains some carried out the most efficient tuning parameters using a Frantz impurities like monazites, spinel, quartz and zircon, as minority magnetic barrier separator type LB-1 for concentrating and mineral . These impurities have a concentration process, refining each mineral phase present in our commercial ilmenite. remaining associated to the co-products or wastes of the This technique is based on the magnetic susceptibility in the industrial process. Therefore, recovery these minerals prior the presence of a magnetic field, adapting the intensity, and the industrial process is economic and environmental interesting. In incline chute angles, side tilt and forward slope . this sense, we have carried out an exhaustive characterisation of Then, the fractions obtained were characterized by determining the ilmenite used in a titanium-dioxide industry, located in the the mineralogical composition (XRD). Moreover, major elements province of Huelva (Spain), which produces pigments by applying were determined by an inductively coupled plasma optical the sulphate process. In this factory, the first residue obtained, emission spectrometry (ICP-OES) by using a Jobin Yvon ULTIMA 2 known as sludge (or undissolved mud), are enriched in titanium system. Trace elements were determined by Inductively Coupled Plasma Mass Spectrometry (ICP-MS) by using an HP4500® system, dioxide (around 50% of TiO2), which represent 5% of the total Ti present in the raw material [11,12]. Also, this sludge is formed by at the Research Central Services, in the University of Huelva, after several refractory mineral phases as unattached ilmenite, rutile, the total dissolution of the samples and its posterior dilution and quartz and zircon coming from the commercial ilmenite used in adaptation for their introduction in the system in 2% nitric acid, the industrial process [13,14]. Currently, there are no economic following the method of fusion studied by other authors . commercial applications for the sludge. Therefore, to recovery Finally, the morphology, microscopic structure and microscopic composition of the mineral fractions were carried out bySEM these mineral phases for subsequent marketing in different analyses using a JEOL JSM-5410 system, working at 20 kV. It has fields would be a possibility environmentally and economically a backscattered electron detector (BSE), by Tetra Link of Oxford, appropriate. In addition, this waste is stored in a controlled and a dispersive X-ray spectrometer for EDS. landfill repository, which implies a cost of about three million euros for its final elimination (including transportation costs). Results and Discussion This waste could be reduced by the optimization of the process and a significant improving in the competitiveness of this industry The mineralogical composition of the ore (commercial ilmenite), obtained by XRD, is characterised by a high concentration of will be produced. In this context, the process optimization is a ilmenite (FeTiO ), 70 ± 6%, compensated by the presence of correct environmental solution to the disposal and economical 3 pseudorutile (Fe Ti O ), 20 ± 3%. Also, is presents, rutile, (7 ± 1%) improving by reducing waste and marketing the minerals. In view 2 3 9 in ac cordance with previous results. of the above, the main objective  of this paper is to specify the physico-chemical characterization of the different mineralogical Tuning method for mineral separation phases presents in the raw material used in a TiO pigment 2 After an exhaustive literature review, the authors don not find industry, and to apply this information in the optimization of the a specific technique and methodology to isolate each mineral industrial process. Consequently, the isolation and recovery the phases in the ilmenite ore. In general the papers present a wide undissolved mineral phases and other impurities before to entry range of adjustment parameters among the methods, but the in the industrial process. most efficient technique is the magnetic separation [18,19]. For
This article is available in: http://www.imedpub.com/resources-recycling-and-waste-management/ 2 2017 Journal of Waste Recycling Vol.2 No.2:5
this reason, it was necessary to tune up a magnetic separation separation is the fraction called “ilmenite fraction” (IF). The rest process, depending on two parameters, intensity (in view of the of the sample was processed according the third separation magnetic susceptibility of each mineral) and angles in the incline (Figure 1) giving the last two fractions, the magnetic material chute in the separator (side tilt and forward slope). The minerals is called “rutile fraction” (RF) and the non-magnetic as “zircon can be mainly classified according to the type of magnetism and fraction” (ZF). magnetic susceptibility (χ ) (ilmenite: ferromagnetism and χ >1; m m Previously, an optimisation in the use of Frantz was performed pseudorutile and rutile: paramagnetism and χ ≈ 10-6; zircon and m according several tests used setting as in the bibliography (test quartz: diamagnetism and χ ≈ -10-6) . m 1-4) and test 5 was proposed by us (Table 1), where the intensity, To carry out the magnetic separation prior the industrial process, side tilt and forward slope were changed in order to achieve samples were firstly sieved obtaining the thick material (particle the optimum group of parameters. Agreeing to the mineral size >250 µm), which was again grounded and completely sieved composition, the most efficient parameters correspond with test smaller than 250 µm. This milling involves no added economic 5 (Table 2), where the ilmenite concentration is around 89%. In cost, since the raw material is grounded with a particle size addition, test 5 also shows the most efficient in the separation <70 µm before entering the industrial process. The magnetic of rutile and zircon, with 58 and 62%, respectively. The other separation method was applied on the fraction between 125 to fractions obtained present a wide variety and concentrations 250 µm, as recommended the Frantz´s manual The fine material of minerals, due to the presence of minerals with similar values (FF) with size smaller than 125 µm and approximately a 7% of of magnetic susceptibility. As explained below, the deposits the total RM, was declined for Frantz separation. In addition, it that may have some mineral species in nature can alter the is necessary to remove the high magnetic fraction prior Frantz results, i.e., minerals that are usually diamagnetic may appear as method (magnetic separation) was applied (Figure 1). According paramagnetic under certain conditions of alteration. to the manual, the most magnetic fraction was rejected to avoid interferences, because its high magnetic susceptibility could Mineral characterization influence in the behaviour of another particles . Fine fraction, (FF), <125 microns, is formed by several mineral The highest magnetic material was obtained by a hand magnet phases as rutile, pseudorutile, ilmenite, zircon, quartz and form the HMF (Hand Magnet Fraction), around a 5% of the total monazite (<5%). On the other hand, (Figure 2) the hand magnet RM. Besides, the magnetic material obtained in first separation fraction (HMF), shown a mineralogical compositions of ilmenite and magnetite (Fe O ) with 30 and 70% respectively, which are (approximately a 16% of the total RM) was saved and later mixed 3 4 with the ilmenite fraction (IF), due to it is composed mostly of the minerals with the highest magnetic susceptibility. Ilmenite ilmenite. Furthermore, the magnetic material obtained in second fraction (IF) present the characteristic peaks of ilmenite and pseudorutile (Figure 2A) , with 89 and 11% respectively (Table 2; test 5). The rutile fraction (RF) corresponds to a mix of minerals such as rutile (58%), zircon (36%) and a minimal presence of pseudorutile. Also, in this fraction a minimum amount of spinel (<5%) is detected (Figure 2B). Moreover, the Table 1: Posed setup parameters. I: Intensity Applied (A), S: Side Tilt (°), F: Forward Slope (°). st nd rd Test 1 Separation 2 Separation 3 Separation I=1.4; S=30; 1 I=0.05; S=30; F=10 I=0.4; S=30; F=10 F=10+S=10; F=5 2 I=0.1; S=25; F=15 I=0.4; S=25; F=15 I=1.4; S=25; F=15 3 I=0.1; S=25; F=10 I=0.3; S=25; F=10 I=1.2; S=25; F=10 4 I=0.05; S=15; F=10 I=0.2; S=15; F=10 I=1.2; S=15; F=10 5 I=0.05; S=12; F=15 I=0.2; S=12; F=15 I=1; S=12; F=15 Table 2: Mineralogical composition (%) crystalline phase by XRD for each fraction obtained by the Frantz after each separation in the different test. I (Ilmenite; Ps (Pseudorutile); S (Spinel); R (Rutile); Z (Zircon); Q (Quartz). Ilmenite Fraction Rutile Fraction Zircon Fraction TEST I Ps I S Ps R Z Q R Z Q 1 61 39 24 N.D. 6 26 27 17 53 33 14 2 62 38 21 N.D. 7 27 27 18 57 25 18 3 72 28 15 N.D. 8 31 27 19 45 38 17 4 64 36 12 N.D. 8 32 30 18 40 41 19 Figure 1 General process by Frantz magnetic separation. 5 89 11 N.D. <5 6 58 36 N.D. 22 62 16 N.D. Not Detected.
© Under License of Creative Commons Attribution 3.0 License 3 2017 Journal of Waste Recycling Vol.2 No.2:5
deposit contains about 45-65% of TiO2 and around 50% of iron, given as FeO . In addition, lower concentrations of Si, Mn, and Zr with a concentration around 1.6, 1.4 and 0.07% respectively are obtained. Also, it presents trace elements like La, Co and Ce (217, 51 and 396 mg kg-1, respectively) as impurities associated to pseudorutile phase. This fact is not unexpected; because it is documented, that pseudorutile presents higher levels of associated trace elements. For example, elements such as Mn, Ce, and Co may substitute Fe or Ti in the original ilmenite lattice, while elements like Al, Si, Th, P and Cr are commonly incorporated into the ilmenite grains during the chemical weathering . For example, the Australian ilmenite concentrates are invariably contaminated with chrome-bearing spinel grains, which are difficult to remove using standard physical separation methods . The FF values are similar to the RM (raw material), except the high concentration of P and Ce, approximately a factor 3 and 2 respectively. These data have been supported further by SEM studies, because appear small particles of monazite (Ce (Ce, La,
Pr, Nd, Th, and Y) PO4). HMF and IF show similar values to RM in most of the major elements, but in iron, HFM presents the highest concentrations with 52% of Fe. According to the mineralogical analysis, because it presents the most magnetic mineral (ilmenite and magnetite), composed mainly by Fe. On the hand, RF presents a lower concentration of Fe (2%) due to the presence of pseudorutile, observed by XRD(Table 2). Taking into account the
B, RF presents a new mineralogical phase, called spinel (MgAl2O4), and logically presents the highest concentration of Al, and Mg with 7.6 and 3.5%, respectively, a factor 10 higher than in the RM. In addition, due to contain certain quantity of zircon mineral, it is
Table 3: Chemical composition of the analysed samples by ICP-OES for the major elements (wt.%) and by ICP-MS for the trace elements (mg/kg). RM (Raw Material); FF (Fine Fraction); HMF (High Magnetic Fraction); IF (Ilmenite Fraction); RT (Rutile Fraction); ZF (Zircon Fraction). Figure 2 Representative DRX spectrum: (A) ilmenite fraction; (B) rutile fraction; (C) zircon fraction. RM FF HMF IF RF ZF Major Elements Fe 36 40 52 38 2 0.46 study of the non-magnetic fraction, called "zircon fraction” (ZF), Ti 37 41 39 39 32 11 shows the characteristic peaks of the three main mineral phases, Al 0.64 0.63 1.4 0.43 7.6 1.3 zircon (62%), but a low content of quartz (22%) and rutile (16%) Si 1.6 1 2.1 1.3 1.4 1.2 (Figure 2C). Finally, it is important to note that these mineral Mg 0.31 1.4 0.81 0.22 3.5 0.11 phases remain in the un-dissolved mud, obtained in the industrial Mn 1.4 1.3 1.3 1.8 0.03 0.01 process, where several species are observed: ilmenite and rutile, Zr 0.07 0.22 0.04 0.03 2.1 4.4 with a percentage of 22% and 34%, respectively, and additionally Trace Elements zircon (12%), quartz (13%), and Fe and Ti oxides (18%) (Fe3Ti3O10) As 37 42 18 39 161 22 [12,13]. The high percentage of rutile and the detection and Cr 464 805 690 420 1000 301 quantification in the mud of the aforementioned mineral phases Sr 476 415 430 512 604 416 (zircon and quartz) cannot be considered as surprising, since P 210 730 260 - 432 403 all of these species are insoluble in sulphuric acid. Therefore, V 960 1089 1200 1000 1000 800 with this previous magnetic separation, these insoluble mineral Co 51 18 - 52 11 2.7 phases can be removed of the final mud. Pb 176 20 - 128 100 22 Major and trace elements Zn 190 100 90 2 440 60 La 217 12 - 67 56 6.9 The chemical analysis by ICP–OES of major and trace elements Th 80 101 45 56 162 17 is shown in Table 3. RM contain mainly two major elements, Ti U 7.7 6.8 5.2 5.4 90 33 and Fe (37% and 36%), as expected, because of typical ilmenite Ce 396 601 - 122 124 16
This article is available in: http://www.imedpub.com/resources-recycling-and-waste-management/ 4 2017 Journal of Waste Recycling Vol.2 No.2:5
no surprising the high concentration of Zr (2.1%), 30 times upper Figure 5 shows a representative SEM and EDX spectrum than in RM sample. ZF fraction shows the lowest concentration corresponding to the ZF (zircon fraction). The morphology is quite in Fe (0.46%), because not present mineral phases containing Fe, complex according SEM image. In relation with EDX, particles as ilmenite or pseudorutile. Nevertheless, it presents the highest contain mainly silicon and titanium with smaller proportions of concentration of Zr (4.4%), 60 times upper than RM. Also shown zirconium and aluminium. For example, particle “A” presents 11% of Ti, being congruent with its mineralogical composition. as major elements zirconium and silicon, compatible with the
Moreover, ZF has the smallest concentration in Mn, a factor 100 presence of zircon mineral, (ZrSiO4), while particle B composed than in the RM, due this element is associated to the presence solely of silicon, corresponds to quartz (SiO2). Rutile particles are of ilmenite . Also, uranium and thorium are accumulated also detected (particle C). mainly in this fraction due to the high concentration of rutile and Due to the complexity of the different phases, a polished probe the presence of monazite, 90 and 160 mg kg-1 for U and Th and of 33 mm (Figure 6) was prepared with RM (raw material) sieved factors 10 and 2 higher than RM. Finally, ZF and RF are around between 125 and 250 microns. These analyses were made to a 2% of the total RM. Taking into account, the quantity of raw (a) confirm the complete range of alteration products andto material used in the factory of Huelva is 142000 t of commercial establish the chemical composition of each phase, (b) determine ilmenite, making up 2840 t of both fractions, RF and ZF. Therefore, the major element constituents, and (c) study the particles in the according the composition shown inTable 3, around of 1200 t of surface and inside. Ti and 150 t of Zr can be remove of the residue obtained in the industrial process, undissolved mud [11-14]. The sample is predominantly composed by ilmenite and its alteration products, with a continuous transition from pure Scanning electron microscopy (SEM) ilmenite, through intermediate alteration phases, such as leached A representative SEM image for the IF can be observed in Figure ilmenite, pseudorutile and leached pseudorutile to secondary 3. EDX spectrum reveals the grains contain major elements as iron rutile . Also, there are many types and shapes of particles, and titanium, agree XRD data, showing the typical composition of where some of them reveal its internal shape, (Figure 6A-6C). A separate study of each different areas, dark (zone 1) and shiny ilmenite particle (FeTiO3), 47% of FeO and 53% of TiO2 . A detailed SEM analysis allows us to know the morphology, formed (zone 2) was conducting. In addition, a third zone (grey area) mainly by ilmenite particles with pseudotabular morphologies. appears in some cases, demonstrating that the grains contain Other ilmenite grains present rhombohedra and tabular different concentrations of iron, titanium, aluminium and silicon morphology, and very uniform composition (Figure 3A), being Ti and Fe the main elements with traces of Mn. On the other hand, the particle "B" is formed by three-quarters of titanium anda quarter of iron (Figure 3B), in agreement with a mineral known as pseudorutile (Fe2Ti3O9) . Finally, extremely shiny microscopic particles were detected in a low proportion (Figure 3C). These particles give a typical heavy metal mineral composition (Nb, Ce, and Th), corresponding to the rare earth metals: cerium, lanthanum and thorium, associated with a mineral phosphate group, called monazite . RF shows a high heterogeneity (Figure 4) in accordance with the morphology. In the EDX spectrum, grains mainly contain Zr, Si, Ti and Al, corresponding to zircon (ZrSiO4), rutile (Figure 4A) (TiO2) and spinel, respectively. In addition, low iron concentration is present, consistent with the presence of pseudorutile. A specific analysis by SEM-EDX, shown that Figure 4A is majority composed by titanium, with a remainder of iron, according to the typical composition of rutile (>90 wt.% TiO2) . Smaller particles (around 150 µm) are also observed, with a high heterogeneous morphology and composition (Figure 4B), containing mainly aluminium and small proportions of silicon, titanium and iron content. This figure shows a typical spectrum of aluminium silicate, corresponding with the minerals group known as spinel. In this fraction appears, as in the ilmenite fraction (IF), the Figure 3 Representative SEM (BSE) image of the “ilmenite fraction” presence of pseudorutile (particle C). Moreover, another mineral sample and EDX spectrum. (A) SEM (BSE)-EDX analysis of is observed, particle D, containing major elements as zirconium a specific ilmenite particle. (B) SEM (BSE)-EDX analysis of a and silicon, with similar values to the typical particle of zirconium specific pseudorutile particle. (C) SEM (BSE)-EDX analysis of a specific monazite particle. silicate (ZrSiO4), 67% to 33% of SiO2 and ZrO2 .
© Under License of Creative Commons Attribution 3.0 License 5 2017 Journal of Waste Recycling Vol.2 No.2:5
Environmental and economical implications According the different fractions obtained during this procedure, some minerals with economical interest are isolated and can be removed prior the industrial process. So, taking into account, the 142000 tons of raw material (RM) used per year in the factory of Huelva. Fine fraction, 7% of total RM, presents mineral like monazite (<5%), making up 9940 tons of FF and around of 497 tons of monazite. Furthermore, the hand magnet fraction (HMF), about 5% of the total RM, is formed mostly by magnetite (70%), making up 7100 tons of HMF and 4970 tons of magnetite. Finally,from RF and ZF, a 2% of the total RM, making up 2840 tons of both fractions. Therefore, around of 60 tons of spinel and 923 tons zircon can be obtained from both fraction, respectively. On the other hand, the Zr and Rutile fraction can be mixed and subsequently treated with HCl to extract the remaining Ti or directly used as raw material in the process via chloride. The zircon and spinel are not affected by the acid attack achieving the separation of these elements from the removed Ti.
Figure 4 Representative SEM (BSE) image of the “rutile fraction sample (backscattered secondary electron mode) and EDX spectrum. (A) SEM BSE-EDX analysis of a specific rutile particle. (B) SEM BSE-EDX analysis of a specific spinel particle. in each area. The difference in iron concentration occurs due to the weathering of the ore, which leaches out the iron from the ilmenite lattice leaving a Ti rich region . Furthermore, zircon can also vary its magnetic susceptibility depending on the composition, according to its presence in both RF (rutile fraction) as ZF (zircon fraction). Pedogenic index presented by zircon, leads us to assume it is weather-proof. However, this assumption has not tested, features appear to be evidence of wear in zircon produced by the mobility of Zr. This evidence is similar to other researchers besides zircon can present impurities by the intrusion of another mineral, Figure 7B. Zircon is formed mainly by zirconium and silicon, zone 1 (light grey) and presents an impurity inside the particle, zone 2 (dark grey). This impurity is formed by titanium and iron, but the iron content Figure 5 Representative SEM (BSE) image of the “zircon fraction is higher than a typical ilmenite particle [33,34]. As explained sample (backscattered secondary electron mode) and before, diamagnetic mineral may appear as paramagnetic under EDX spectrum. (A) SEM BSE-EDX analysis of a specific certain conditions of alteration, hindering their total isolation zircon particle. (B) SEM BSE-EDX analysis of a specific quartz particle. (Figure 7).
This article is available in: http://www.imedpub.com/resources-recycling-and-waste-management/ 6 2017 Journal of Waste Recycling Vol.2 No.2:5
Also, in this procedure about of 86% of the RM forms the Ilmenite fractions minerals, which cannot be dissolved in the digestion fraction, which around 89% is formed by ilmenite mineral. It step, come in the industrial process and therefore in the final makes up 122120 tons of IF and approximately 108687 tons of residue (undissolved mud). The magnitude of this generated pure ilmenite. waste is around 30,000 tons per year, which until now have not had any use, and therefore it is disposed of in an authorized In the experimental protocol proposed in this study, with some waste repository. Therefore, this procedure would not only help adjustments in this separation process, as well as with the to optimize the industrial process but could also reduce the use of other ore separation technologies, most of the mineral potential risk of pollution from the undissolved mud stack to the can be isolate prior to the industrial process. Avoiding these environment. Summary and Conclusions The general results obtained in this work were firstly to develop a magnetic method to isolate the mineral phases in the titanium dioxide industry ore (commercial ilmenite), being test number 5 the set parameters more efficiency according separation, see Table 2. The results obtained with our "setting" are better than these obtained following the Frantz methodology (test 1-4). Secondly, physico-chemical characterization of each mineral from the ore was carried out. It is composed of ilmenite and its alteration products (ilmenite unchanged, leached ilmenite, pseudorutile, leached pseudorutile and rutile). Only three different diffraction patterns can be detected among allthe different phases of transformation ilmenite, pseudorutile and rutile, by XRD. Leached ilmenite and leached pseudorutile are transitional metastable phases and show the same structure as the respective parent minerals, ilmenite and pseudorutile, until the structure breaks down completely. According SEM result, these particles were originally pure particles of ilmenite, due to the weathering fracture lines have formed inside the grains. Subsequently, located in these fractures, occurs an alteration and transformation of the original mineral, appearing different Figure 6 Representative SEM (BSE) image of the polished probe “raw material sample (secondary electron mode). (A) transformation stages. With the progressive loss of iron, it SEM-EDX analysis of specific particle A. (B) SEM-EDX is transformed from ilmenite (shiny areas), to pseudorutile analysis of a specific pseudorutile particle B. (C) SEM-EDX (intermediate areas) and lastly with the total loss, to rutile (dark analysis of a specific pseudorutile particle C. areas).
Figure 7 SEM-EDX analysis of: (A) zircon particle 1; (B) zircon particle 2.
© Under License of Creative Commons Attribution 3.0 License 7 2017 Journal of Waste Recycling Vol.2 No.2:5
In more detail, our results indicate that the main raw material this procedure optimizes the industrial process and could also used (ilmenite) has a variable mineralogical and elemental reduce the waste generation (undissolved mud) and the potential composition. The concentrate contains small amounts (1.5-2%) environment risk. of others minerals potentially economics (monazite is associated with the fine fraction, spinel with the rutile fraction, quartz with Acknowledgements the zircon fraction, etc.). The minerals contained in the ilmenite This research has been partially supported by the Government are not pure (physical mixes of them), implies the fact that it is impossible to isolate 100% the different mineral fractions initially of Andalusia´ s Project “Characterization and modelling of the present in the raw material. phosphogypsum stacks from Huelva for their environmental management and control” (Ref.: RNM-6300). Dr. M. Contreras According the different fractions obtained during this procedure, expresses her gratitude for the contract by The Fellowship some minerals with potential economic interest can be removed Training Program of the University Teaching Staff, reference from the ore prior the industrial process, like monazite in FF, AP2010-2746, financed by the Spanish Ministry of Education, magnetite in HMF, spinel in RF, and zircon in ZF. Obtaining an Culture and Sport (MECD). ilmenite ore mostly formed by ilmenite mineral. Furthermore,
15 Gázquez MJ, Bolívar JP, Garcia-Tenorio R (2007) A Review of the References Production Cycle of Titanium Dioxide Pigment. Mater Sciand 1 Zhang W, Zhu Z, Cheng CY (2011) A Literature Review of Titanium Applications 441: 458. Metallurgical Processes. Hidrometallurgy 177: 188. 16 Augusto PA, Augusto P, Castelo-Grande T (2002) Magnetic classification. 2 McNulty GS (2007) Production of Titanium Dioxide. Plenary Lecture. Miner Eng 35: 43. NORM V International Conference, Sevilla. 17 Mantero J, Lehritane M, Hurtado S (2010) Radioanalytical 3 Rosebaum JB (1982) Titanium Technology Trends. J Miner Met and Determination of Actinoids in Refractory Matrices by Alkali Fusion. J Mater Society 76: 80. Radioanal Nucl Chem 557: 563. 4 Stwertka A (1998) Guide to the Elements. Revised Edition, Oxford 18 Frantz Co SG (1965) Assembly, Installation, Operation and Maintenance University Press, London. Instruction. Frantz Magnetic Separator. 5 Williams VA (1990) WIM 150 Detrital Heavy Mineral Deposit. In: 19 Cui Z, Liu Q, Etsell TH (2002) Magnetic Properties of Ilmenite, Hughes FE (ed.) Geology of the Miner Deposits. Hematite and Oilsand Miner After Roasting. Miner Eng 1121: 1129. 6 Adams R (1994) The World Market for TiO2 Feedstocks. Miner 20 Hutchison SC (1974) Laboratory Handbook of Petrographic Industry International 9: 14. Techniques. Wiley and Sons edit. 7 Barksdale J (1966) The Roland Press Company, New York. Titanium, 21 Li C, Liang B, Guo LL (2007) Dissolution of Mechanically Active Its Occurrence, Chemistry, and Technolog, (2ndedn). Panzhihua Ilmenites in Dilute Solutions of Sulphuric Acid. 8 Mucke A, Bhadra Chaudhuri JN (1991) The Continuous Alteration of Hydrometallurgy 1: 10. Ilmenite through Pseudorutile to Leucoxene. Ore Geology Reviews 2: 44. 22 Chernet T (1999) Mineralogical and Textural Constrainst on Miner Processing of the Koivusaaarenneva Ilmenite Ore, Kälviä, Western 9 Pownceby MI (2010) Alteration and Associated Impurity Element Finl and. Int J Miner Process 153: 165. Enrichment in Detrital Ilmenites from the Murray Basin, Southeast Australia: A Product of Multistage Alteration, Australian Journal of 23 Pownceby MI, MacRae CM, Wilson NC (2007) Miner Characterisation Earth Sci 243: 258. by EPMA Mapping. Miner Eng 444: 451. 10 Gupta CK, Krishnamurthy N (2004) Extractive Metallurgy of Rare 24 Pownceby IM (2005) Compositional and Textural Variation in Detrital Earths. CRC Press, London. Chrome-spinels from the Murray Basin, Southeastern Australia. Mineralogical Magazine 191: 204. 11 Contreras M, Gázquez MJ, García-Díaz (2013) Valorisation of Waste Ilmenite Mud in the Manufacture of Sulphur Polymer Cement. 25 Kalinkina EV, Kalinkin AM, Forsling W (2001) Sorption of Atmospheric Journal of Env Management 625: 630. Carbon dioxide and Structural Changes of Ca and Mg Silicate Miner During Grinding: I. Diopside. Int J Miner Process 273: 288. 12 Contreras M, Martín MI, Gázquez MJ (2013) Valorisation of Ilmenite Mud Waste in the Manufacture of Commercial Ceramic. Construction 26 Pownceby MI, Sparrow GJ, Fisher-White MJ (2008) Mineralogical and Building Materi 31: 40. Characterisation of Eucla Basin Ilmenite Concentrates - First Results from a New Global Resource. Miner Eng 587: 597. 13 Gázquez MJ, Bolívar JP, García-Tenorio R (2009) Physicochemical Characterization of Raw Materials and Co-products from the 27 Teufer G, Temple AK (1996) Pseudorutile – A New Miner Intermediate Titanium Dioxide Industry. J of Hazardous Mater 1429: 1440. Between Ilmenite and Rutile in the Alteration of Ilmenite. Nature 14 Gázquez MJ, Mantero J, Bolívar JP (2011) Physico-chemical and 179: 181. Radioactive Characterization of TiO2 Undissolved Mud for its 28 Jha AL (2009) Selective Separation of Rare Earths and Impurities from Valorization. J Hazardous Mater269: 276. Ilmenite Ore by Addition of K+ and Al3+ ions. Hydrometallurgy 254: 261.
This article is available in: http://www.imedpub.com/resources-recycling-and-waste-management/ 8 2017 Journal of Waste Recycling Vol.2 No.2:5
29 Mackowski SJ, Reaveley BJ, Woodcock JT (1993) Synthetic Rutile 32 Temple AK (1966) Alteration of Ilmenite. Economic Geology 695: 714. Production at Tiwest Joint Venture. In: Chandala WA (ed.) Australasian 33 Berrow ML, Wilson MJ, Reaves GA (1978) Origin of Extractable Mining and Metallurgy, The Sir Maurice Mawby Memorial Volume, Monograph Series Monograph No. 19, The Australasian Institute of Titanium and Vanadium in the A Horizons of Scottish Podzols. Mining and Metallurgy, Carlton 1304: 1308. Geoderma 89: 103. 30 Tejan-Kella MS, Fitzpatrick RW, Chittleborough DJ (1991) Scanning 34 Bull PA, Goudie AS, Williams DP (1987) Colluvium: A Scanning Electron Microscope Study of zircons and Retiles from a Podzol Electron Microscope Analysis of a Neglected Sediment type. In: Chronosequence at Cooloola, Queensland, Australia. Catena 11: 30. Marshall JR (ed.) Clastic Particles - Scanning Electron Microscopy and Shape Analysis of Sedimentary and Volcanic Clastics. Reinhold, New 31 Chernet T (1999) Applied Mineralogical Studies on Australian Sand York 16: 35. Ilmenite Concentrate with Special Reference to its Behaviour in the Sulphate Process. Miner Eng 485: 495.
© Under License of Creative Commons Attribution 3.0 License 9